Large structural transformation and ferromagnetic ordering in a coordination polymer with a two-dimensional square-planar lattice, bis(glycolato)copper(ii)
Yoneyama, Shota; Kodama, Takeshi; Kikuchi, Koichi; Kawabata, Yohei; Kikuchi, Kentaro; Ono, Toshio; Hosokoshi, Yuko; Fujita, Wataru; CrystEngComm 15 (2013) 10193–; doi:10.1039/c3ce41806e

data_7211483
_publ_section_title
;
 Large structural transformation and ferromagnetic ordering in a
 coordination polymer with a two-dimensional square-planar lattice,
 bis(glycolato)copper(ii)
;
_journal_issue                   47
_journal_name_full               CrystEngComm
_journal_page_first              10193
_journal_paper_doi               10.1039/c3ce41806e
_journal_volume                  15
_journal_year                    2013
_chemical_formula_moiety         'C4 H6 Cu O6'
_chemical_formula_sum            'C4 H6 Cu O6'
_chemical_formula_weight         213.63
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_Int_Tables_number      14
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_cell_angle_alpha                90.0000
_cell_angle_beta                 107.141(8)
_cell_angle_gamma                90.0000
_cell_formula_units_Z            2
_cell_length_a                   5.0908(8)
_cell_length_b                   8.6939(12)
_cell_length_c                   7.7300(14)
_cell_measurement_reflns_used    900
_cell_measurement_temperature    249
_cell_measurement_theta_max      27.40
_cell_measurement_theta_min      3.60
_cell_volume                     326.93(9)
_computing_cell_refinement       'CrystalClear-SM Expert 2.0 r4'
_computing_data_collection
'CrystalClear-SM Expert 2.0 r4 (Rigaku, 2009)'
_computing_data_reduction        'CrystalClear-SM Expert 2.0 r4'
_computing_molecular_graphics    'CrystalStructure 4.0'
_computing_publication_material  'CrystalStructure 4.0 (Rigaku, 2010)'
_computing_structure_refinement  'SHELXL97 (Sheldrick, 2008)'
_computing_structure_solution    SIR97
_diffrn_ambient_temperature      249
_diffrn_detector_area_resol_mean 14.706
_diffrn_measured_fraction_theta_full 0.996
_diffrn_measured_fraction_theta_max 0.996
_diffrn_measurement_device_type  'Rigaku Mercury'
_diffrn_measurement_method       \w
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71075
_diffrn_reflns_av_R_equivalents  0.0282
_diffrn_reflns_limit_h_max       6
_diffrn_reflns_limit_h_min       -6
_diffrn_reflns_limit_k_max       7
_diffrn_reflns_limit_k_min       -11
_diffrn_reflns_limit_l_max       9
_diffrn_reflns_limit_l_min       -10
_diffrn_reflns_number            2360
_diffrn_reflns_theta_full        27.42
_diffrn_reflns_theta_max         27.42
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    3.319
_exptl_absorpt_correction_T_max  0.718
_exptl_absorpt_correction_T_min  0.528
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'REQAB (Rigaku, 1998)'
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    2.170
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       unknown
_exptl_crystal_F_000             214.00
_exptl_crystal_size_max          0.400
_exptl_crystal_size_mid          0.100
_exptl_crystal_size_min          0.100
_refine_diff_density_max         0.290
_refine_diff_density_min         -0.330
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.183
_refine_ls_hydrogen_treatment    refxyz
_refine_ls_number_parameters     64
_refine_ls_number_reflns         743
_refine_ls_number_restraints     0
_refine_ls_R_factor_gt           0.0255
_refine_ls_shift/su_max          0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w = 1/[\s^2^(Fo^2^)+(0.0280P)^2^+0.0783P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_ref         0.0640
_reflns_number_gt                647
_reflns_number_total             743
_reflns_threshold_expression     F^2^>2.0\s(F^2^)
_cod_data_source_file            c3ce41806e.txt
_cod_data_source_block           13042302_250K01
_cod_original_cell_volume        326.93(10)
_cod_database_code               7211483